International Journal of Engineering and Science Invention (IJESI)
International Journal of Engineering Science Invention
ISSN (Online): 2319 – 6734, ISSN (Print): 2319 – 6726
www.ijesi.org Volume 2 Issue 10ǁ October2013 ǁ PP.62-68
Polypropylene and Polystyrene Waste Plastics Mixture to Diesel
Fuel for Truck/Bus Engines
Mohammad Mamunor Rashid, Moinuddin Sarker *,
Natural State Research, Inc., Department of Research and Development, 37 Brown House Road (2 nd Floor),
Stamford, CT-06902, USA
Phone: (203) 406-0675, Fax: (203) 406-9852
ABSTRACT:Polypropylene and polystyrene waste plastics mixture to diesel grade fuel production process
was performed in to laboratory scale. Experimental main goal was diesel fuel collection by using fractional
distillation process. Experimental temperature was use up to 400 ºC and fractional distillation purposed
temperature was used 285 ºC. Under laboratory fume hood and batch process experiment was perform without
catalyst and experimental run time was 6 hours. Produced fuel density is 0.81 g/ml. Liquid fuel was analysis by
using GC/MS and compounds data table shown below table in result and discussion section.
KEYWORDS: Polypropylene, polystyrene, diesel fuel, hydrocarbon, GC/MS
The amount of waste plastics discarded each year is constantly increasing and is causing serious
pollution problems. If this material can be chemically recycled, this material will become a cheap and abundant
source for useful chemicals and energy. Among various recycling methods, the chemical method which converts
waste plastics to useful hydrocarbons, has been recognized as a promising approach. In view of their
versatility and relatively low cost, the consumption of plastic materials has been growing steadily, although the
disposal of waste plastics constitutes a severe environmental problem due mainly to their chemical inertness.
While polymers recycling is a requirement to mitigate their impact on the environment , various tertiary
recycling processes are attractive, since they produce valuable chemicals or fuels [3, 4]. Considering
polyolefins, polyethylene and polypropylene have a massive production and consumption in a large number of
applications. Plastic materials production has reached global maximum capacities levelling at 260 million
tonnes in 2007, where in 1990 the global production capacity was estimated at an 80 million tonnes . It is
estimated that production of plastics worldwide is growing at a rate of about 5% per year . Over the past
seventy years, the plastic industry has witnessed a drastic growth, namely in the production of synthetic
polymers represented by polyethylene (PE), polypropylene (PP), polystyrene (PS), polyethylene terephthalate
(PET), polyvinyl alcohol (PVA) and polyvinyl chloride (PVC). Plastics also contribute to our daily life
functions in many aspects. Household goods nowadays are mainly composed of plastic or plastic reinforced
materials, from packaging, clothing, appliances and electrical and vehicle equipments, to insulations, industrial
applications, greenhouses, automotive parts, aerospace and mulches.
High temperature pyrolysis and cracking of waste thermoplastic polymers, such as polyolefines,
polyethylene (PE), polypropylene (PP) and polystyrene (PS), are well- known and environmentally accepted
methods of their utilisation. This group of processes embraces thermal pyrolysis and cracking, catalytic cracking
and hydrocracking in the presence of hydrogen. Pyrolysis is the typical chemical recycling process, enabling
production of monomers, mainly ethylene, propene and butene from waste plastics. In case of cracking
processes, their main products are fuels fractions, gaseous hydrocarbons and liquid mixtures of hydrocarbons
boiling in the range of temperatures ~35–360 ºC (gasoline and light gas oils) as well as the solid carbon
residues, similar to coke. Some researcher experimental results of application of various acidic catalysts was
use for fuel production, such as silica–alumina, zeolites (HY, HZSM-5, mordenite) or alkaline compounds such
as ZnO, CaO and K2O [10–13]. In this present technology diesel fuel production was perform without catalyst
with fractional distillation process and temperature was use only 285 ºC for diesel fuel collection.
MATERIALS AND METHOD
Polypropylene and Polystyrene waste plastics mixture to fuel production process was perform in to
laboratory scale. Two step processes experiment was perform without catalyst and waste materials was use for
experiment 250 gm. PP and PS waste ratio was 50:50. 1st step process temperature was use up to 400 ºC and 2nd
62 | Page
Polypropylene And Polystyrene Waste…
step process temperature was use 285 ºC. Pyrex glass was using both steps and heat mental, variac
meter was use for temperature controller. Figure 1 is shown fuel process diagram for visual understanding. 1st
step process waste plastic cut into small pieces and places into pyrex glass inside then setup condensation unit
with collection flask. Heat mental was use for waste materials melting purposed and temperature was increased
and decreased by using variac meter. Electrical heat was use for sample meting and glass condensation was use
for vapor condensation without water flow. Usually water is using for condensation cooling purpose but in this
experiment doesn’t required water cooling for condensation. When heat rise up gradually then waste plastics
start to melt then it become slurry then it become a vapor. Vapors are traveled to condensation inside and due to
room temperature inside vapor are become a cool at the end liquid fuel is collected. This product fuel density is
0.89 g/ml. In this process liquid fuel was collected 192.1 g and volume was 217 ml. left over residues was 50.9
gm and light gas was 7 gm. In mass balance calculation percentage showed 76.84 % liquid fuel, residue
20.36% and light gas was 2.8%. Residue percentage is high because polystyrene waste plastic additives
percentage is high. After finished 1st step process then start 2nd step process for fractional process. In 2 nd
fractional process product fuel was fractionation temperature wise and collected diesel grade fuel at 285 ºC.
Liquid 1st step product fuel was fractionation at 285 ºC and collected diesel grade fuel but before get diesel
grade fuel in this process also produce gasoline grade fuel, naphtha grade fuel and aviation or jet grade fuel.
Experimental process main goal was diesel grade fuel collection. 192.1 gm liquid fuel to taken out 12.5 gm for
analytical analysis to determine 1st step fuel compounds structure. For 2nd step distillation process liquid fuel
was use 179.6 gm for collected diesel grade fuel. Product diesel grade fuel density is 0.81 g/ml. 179.6 gm liquid
to diesel grade fuel was 35 gm and volume was 43 ml. During fractional distillation production period other fuel
was produced such as gasoline grade, naphtha grade, aviation or jet grade and fuel oil grade. Light gas was
produce 32.7 gm and left over residue was 11.0 gm. Other grade fuel was produce 100.9 gm. In percentage
calculation 2nd step process diesel grade fuel collection was 19.49%. Fuel was thicker and light yellow color.
[1. Electric Cord, 2. Variac, 3. Heat Mantle, 4. Sample (Waste Plastic PP and PS), 5. Boiling Flask, 6.
Condensation Unit, 7. Water Inlet, 8. Water Outlet, 9. Open & Close System Bulb, 10. Electric Cord, 11. Variac,
12. Heat Mantle, 13. Fuel (For Fraction), 14. Boiling Flask, 15. Condensation Unit, 16. Water Inlet, 17. Water
Outlet, 18. Ring Cork, 19. NSR Fuel (Diesel Collection), 20. Collection Flask, 21. Lighter Gas Escape Path]
Figure 1: PP and PS waste plastic fuel to diesel fuel production process.
63 | Page
Polypropylene And Polystyrene Waste…
Benzeneacetic acid, 4pentadecyl ester
Cyclopentane, 1,1'-[3-(2cyclopentylethyl)-1,5pentanediyl]bisBenzene, [6-cyclopentyl-3(3-cyclopentylpropyl)hexyl]9-Octadecenoic acid (Z)-,
Benzene, [3-(2cyclohexylethyl)-6cyclopentylhexyl]Indeno[2,1-a]indene, 5,10dihydro(2,3Diphenylcyclopropyl)methyl
phenyl sulfoxide, transBenzene, 1,1'-[2-methyl-2(phenylthio)cyclopropyliden
A PP and PS mixture waste plastic to diesel fuel production was fractional distillation process. Product fuel was
analysis by GC/MS to determine compound structure and carbon range present into fuel. GC/MS fuel
chromatogram analysis result graph shown figure 2, and carbon range compounds data table shown into table 1.
Product fuel carbon range showed C6 to C25. Product fuel has hydrocarbon compounds including aromatic
group, oxygenated, alcoholic group, and halogenated group because waste plastic has additives. During
production period some negligible percentage of additive are comes out with fuel. All compounds were traced
from chromatogram based on NIST library with retention time (t) and trace mass (m/z). All compounds peak
intensity is not same some compounds peak intensity is small, some compounds peak intensity is medium and
some compounds peak intensity is large. Starting compounds peak intensity is small and end compounds peak
intensity is small. Benzene group compounds are present in this fuel because raw materials were used
polystyrene waste plastic. Polystyrene waste plastic has benzene group compounds. Diesel grade fuel production
purposed temperature was used 285 ºC. GC/MS analysis compounds are appeared small number carbon to large
number carbon wise. GC/MS analysis compounds data table 1 showed 104 compounds determined with
retention time, trace mass, compounds formula, molecular weight, probability percentage and NIST library
Initial compounds is 2-methyl-Pentane (C6H14) (t=1.95, m/z=43) molecular weight is 86 and
probability percentage is 45.8%, then 2,4-dimethyl-1-Pentene (C7H14) (t=2.43, m/z=56) molecular weight is 98
and probability percentage is 48.8%, Toluene (C7H8) (t=3.74, m/z=91) molecular weight is 92 and probability
percentage is 38.2%, 1,3,5-trimethyl-Cyclohexane (C9H18) (t=4.71, m/z=69) molecular weight is 126 and
probability percentage is 44.1%, 3,3,5-trimethyl-Cyclohexene (C9H16) (t=5.29, m/z=109) molecular weight is
124 and probability percentage is 32.6%, 1-Nonene (C9H18) (t=6.32, m/z=43) molecular weight is 126 and
probability percentage is 6.36 %, 4-methyl-Nonane (C10H22) (t=6.73, m/z=57) molecular weight is 142 and
probability percentage is 25.0%, 2-methyl-3-methylene-Nonane (C11H22) (t=7.23, m/z=69) molecular weight is
154 and probability percentage is 8.39%, 3,3-dimethyl-Octane (C10H22) (t=7.50, m/z=43) molecular weight is
142 and probability percentage is 6.93%, (E)- 5-Undecene (C11H22) (t=8.05, m/z=56) molecular weight is 154
and probability percentage is 8.37%, 2-butyl-1-Octanol (C12H26O) (t=8.26, m/z=43) molecular weight is 186
and probability percentage is 5.04%, 4,6,8-trimethyl-1-Nonene (C12H24) (t=8.96, m/z=43) molecular weight is
168 and probability percentage is 7.66%, (1,3-dimethyl-3-butenyl)-Benzene (C12H16) (t=10.16, m/z=105)
molecular weight is 160 and probability percentage is 29.4%, 5-butyl-4-Nonene (C13H26) (t=10.24, m/z=69)
molecular weight is 182 and probability percentage is 6.47%, 4,6-dimethyl-Dodecane (C14H30) (t=10.94,
m/z=43) molecular weight is 198 and probability percentage is 11.1%, E-2-Hexadecacen-1-ol (C16H32O)
(t=11.48, m/z=83) molecular weight is 240 and probability percentage is 3.63 %, (Z)-3-Hexadecene (C16H32)
(t=12.55, m/z=43) molecular weight is 224 and probability percentage is 3.73%, 2,5,5-Trimethyl-3-phenylcyclohexanone (C15H20O) (t=13.39, m/z=145) molecular weight is 216 and probability percentage is 27.8%,
2,3,5,8-tetramethyl- Decane (C14H30) (t=14.21, m/z=43) molecular weight is 198 and probability percentage is
67 | Page
Polypropylene And Polystyrene Waste…
9.15%, 1-Nonadecanol (C19H40O) (t=14.64, m/z=83) molecular weight is 284 and probability percentage is
3.43%, bis-1,1'-[3-(3-cyclopentylpropyl)-1,5-pentanediyl] Benzene (C25H34) (t=16.09, m/z=91) molecular
weight is 334 and probability percentage is 19.4%, 2,6,10-trimethyl-Tetradecane (C17H36) (t=16.41, m/z=43)
molecular weight is 240 and probability percentage is 7.38%, bis-1,1'-[3-(2-cyclopentylethyl)-1,5pentanediyl]Cyclopentane (C22H40) (t=17.99, m/z=69) molecular weight is 304 and probability percentage is
4.51%, [3-(2-cyclohexylethyl)-6-cyclopentylhexyl]- Benzene (C25H40) (t=18.64, m/z=69) molecular weight is
340 and probability percentage is 8.93%, and so on. Product fuel has large number of hydrocarbon compounds
for that reason this can use only bus, truck.
Polystyrene waste plastic and polypropylene waste plastic mixture to diesel fuel production process
was two stem processes. 1st step process PP and PS waste plastic mixture to produce fuel, and produce fuel
further fractional distillation process was separated diesel grade fuel without using catalyst. Product fuel was
analysis by GC/MS and compounds start is C6 to C25 and product fuel has hydrocarbon compounds including
aromatic group. Aromatic compounds are present such as Toluene (C7H8), Ethylbenzene (C8H10), (1methylethyl)-Benzene (C9H12), 1,2,3-trimethyl-Benzene (C9H12), butyl-Benzene (C10H14), (3-methyl-1methylenebutyl)-Benzene (C12H16), [6-cyclopentyl-3-(3-cyclopentylpropyl)hexyl]-Benzene (C25H40) and
many more. Product fuel is not igniting because product fuel hydrocarbon compounds heaver compounds
mixture. Heavy hydrocarbon compounds can use heavy engine such as truck or bus.
The authors acknowledge the support (Financial) of Dr. Karin Kaufman, the founder and sole owner of
Natural State Research, Inc. The author also acknowledges the valuable contributions NSR laboratory team
members during the preparation of this manuscript.
Takao Masuda, Tatsuhiko Kushino, Toshihiro Matsuda, Shin R. Mukai, Kenji Hashimoto, Shu-ichi Yoshida; Chemical
recycling of mixture of waste plastics using a new reactor system with stirred heat medium particles in steam atmosphere,
Chemical Engineering Journal 82 (2001) 173–181
G. Scott, Polym. Degrad. Stabil. 68 (2000) 1.
K. Fouhy, I. Kim, S. Moore, E. Culp, Chem. Eng. 100 (1993) 30.
S. Shelley, K. Fouhy, S. Moore, Chem. Eng. 99 (1992) 30.
G. de la Puente, C. Klocker, U. Sedran, Conversion of waste plastics into fuels Recycling polyethylene in FCC, Applied
Catalysis B: Environmental 36 (2002) 279–285
Valavanidis A, Iliopoulos N, Gotsis G, Fiotakis K. Persistent free radicals, heavy metals and PAHs generated in particulate soot
emissions and residue ash from controlled combustion of common types of plastic. J Hazard Mater 2008;156:277–84.
APC, American Plastics Council. Facts and figures, Arlington VA 22209. Technical paper. Available at:
S.M. Al-Salem*, P. Lettieri, J. Baeyens, The valorization of plastic solid waste (PSW) by primary to quaternary routes: From reuse to energy and chemicals, Progress in Energy and Combustion Science 36 (2010) 103–129
Jerzy Walendziewski, Continuous flow cracking of waste plastics, Fuel Processing Technology 86 (2005) 1265– 1278
Y. Uemichi, M. Hattori, T. Itoh, J. Nakamura, M. Sugioka, Deactivation behaviors of zeolite and silica– alumina catalysts in the
degradation of polyethylene, Ind. Eng. Chem. Res. 37 (1998) 867– 872.
W. Ding, L. Liang, L.L. Anderson, Thermal and catalytic degradation of high density polyethylene and commingled postconsumer plastic waste, Fuel Process. Technol. 51 (1997) 47–62.
Z. Zhibo, S. Nishio, Y. Morioka, A. Ueno, H. Ohkita, Y. Tochihara, Thermal and chemical recycle of waste polymers, Catal.
Today 29 (1996) 303– 308.
S. Kargfz, T. Karayildirim, S. Ucar, M. Yuksel, J. Yanik, Liquefaction of municipal waste plastics in VGO over acidic and nonacidic catalysts, Fuel 82 (4) (2003) 415– 423.
68 | Page